NANO-GRAINED STEELS PRODUCED BY VARIOUS SEVER PLASTIC DEFORMATION 2014. 1. 28.¢ The...
Embed Size (px)
Transcript of NANO-GRAINED STEELS PRODUCED BY VARIOUS SEVER PLASTIC DEFORMATION 2014. 1. 28.¢ The...
NANO-GRAINED STEELS PRODUCED BY VARIOUS SEVER PLASTIC DEFORMATION PROCESSES
M.Umemoto*, Y.Todaka and K.Tsuchiya
Department of Production Systems Engineering, Toyohashi University of Technology,
Toyohashi, Aichi 441-8580
The formation of nanocrystalline structure (NS) in steels by various severe plastic deformation processes, such as ball milling, a ball drop test, particle impact deformation, drilling, sliding wear, ultrasonic shot peening and air blast shot peening was studied. Nanograined regions were produced near the specimen surface. The deformation induced nanograined regions have the following common specific characteristics: 1) with grains smaller than 100 nm, 2) extremely high hardness, 3) dissolution of cementite when it exist and 4) no recrystallization and slow grain growth by annealing. It was suggested that the most important condition is to impose a strain larger than about 7.
Keywords: nanocrystal, severe plastic deformation, steels, shot peening
Large efforts have been devoted to refine grains of materials since ultrafine-grained materials have often superior mechanical and physical properties to those of coarse-grained counterparts. Among the various methods proposed to obtain nanograined materials (grain size smaller than 100 nm) [1,2], severe plastic deformation [3,4] has received the largest attention due to the simplicity and applicability for all class of materials. Figure 1 shows representative severe plastic deformation processes to produce nanocrystalline structure (NS):
Fig.1 Vario * Correspon
Ball drop test
Particle impact deformation
～ ～～ ～
High pressure torsion
Ultrasonic shot peening Air blast shot peeningDrilling Sliding wear
us severe plastic deformation processes to produce nanograined structure ding Author. email@example.com
Ultrafine Grained Materials III Edited by Y.T. Zhu, T.G. Langdon, R.Z. Valiev, S.L. Semiatin, D.H. Shin, and T.C. Lowe. TMS (The Minerals, Metals & Materials Society), 2004
ball milling [5,6], high pressure torsion , a ball drop test , particle impact deformation , drilling, sliding wear , ultrasonic shot peening  and air blast shot peening [9,12]. In the present study the microstructure evolutions in steels by these methods (except high pressure torsion) were observed. Focusing on iron and steels, the amount of strain, strain rate to produce NS are discussed.
The materials used in the present study were Fe-0.10C (Fe-0.099C-0.20C-1.37Mn in
mass% hereafter, martensite structure), Fe-0.15C (Fe-0.15C-0.35Si-1.24Mn, ferrite+cementite), Fe-0.80C (Fe-0.800C-0.20Si-1.33Mn, pearlite or spheroidite structure), Fe-3.3Si (Fe-0.027C-3.29Si-0.01Mn, ferrite) and the case hardening SCM420H steel. The details of the experimental conditions of ball milling, a ball drop test, particle impact test and air blast shot peening (ABSP) were described in our previous papers[8,9,13]. The drilling test was performed using a drill of 2.5 mm in diameter with cutting speed of 50 m/min and feed of 0.05 mm/rev. Oil mist was used for coolant. Wear test was performed using a rod sample (15 mm in diameter) and a plate tool (5 mm wide). The tool was made of SKD61 (alloy tool steel for hot dies and hardness of HV 850). A rod specimen was rotated with a speed of 25 rpm (sliding speed of 1 m/s) and rubbed by the tool for 5 mm as is shown in Fig.1. Running methanol (50 cc/min) was used for a coolant. Ultrasonic shot peening (USSP) was performed for 1.8 ks using JIS SUJ2 shot (0.4 mm in diameter). In the experiment, the shots were placed in the chamber vibrated (frequency: 20 kHz, amplitude: 90 µm) by a generator, with which the shots were resonated as is shown in Fig.1. The projection distance was 10 mm. Annealing of nanocrystallized specimens was carried out at 873 K for 3.6 ks by sealing in a quartz tube under a pure Ar protective atmosphere. Specimens were characterized by SEM, TEM and Vickers microhardness tester (load of 0.25 N for 15 s). Specimens for SEM observations were etched by 5 % Nital.
Nanocrystallization by Ball Milling
Figure 2 shows SEM micrographs of the ball milled Fe-0.1C martensite with initial hardness of 3.2 GPa. From the full view of the cross section of a powder (Fig. 2 (a)) two distinct regions are recognized. One is the dark uniform contrast region with several tens of μ m thick observed near the surface of powder and the another is the bright contrast region observed interior of the powder with deformed martensite morphology. The hardness of dark contrast region (8.8 GPa) is much higher than that of bright contrast region (3.9 GPa) as shown in Fig. 2 (b). The boundaries between these two types of regions are clear and sharp. There is no intermediate structure between these two regions. TEM observation (shown below) revealed that the dark contrast area corresponds to nanograined structured region and the bright contrast area corresponds to dislocated cell structured region, respectively. These two types of structures were observed in all the ball milled carbon steels irrespective of the carbon content (0 ~ 0.9 mass%C) or starting microstructure (ferrite, martensite, pearlite or spheroidite).
8.8 GPa 3.9 GPa
Fig.2 SEM micrographs of Fe-0.10C martensite ball milled for 360 ks. (a) as ball milled and (b) after annealed at 873 K for 3.6 ks.
Nanocrystallization by a Ball Drop Test and particle impact deformation
NS can be produced near the surface of specimens after one or several times of a ball (weight attached) drops. Figure 3 shows a typical dark contrast layer formed in Fe-0.15C with fine grained ferrite structure (Fig.3(a)) and in Fe-0.80C specimen with pearlite structure (Fig.3(b)), respectively. The microhardness of the dark contrast layer is much higher than the adjacent region with deformed structure.
Figure 4 shows a typical nanocrystalline layers formed in pearlitic Fe-0.80C specimen after particle impacts at LN2 temperature. The dark contrast layer of about 10 µm thickness observed on the top surface was confirmed as nanocrystalline region by TEM observation. The microhardness of the nanocrystalline region (9.7 GPa) is substantially higher than the subsurface region with deformed structure (4.5 GPa).
Nanocrystallization by drilling and wear
The microstructure along the depth from the surface of drill hole is shown in Fig.5. In the picture the hole is at the top and drilling direction is located horizontally. The specimen used was a case hardening steel (SCM420H). The specimen was carburized and quenched to obtain martensite structure. Uniform contrast layer is seen near the surface. TEM observation revealed that the microstructure close to the surface is equiaxed grains with about 100 nm in diameter. It is considered that the drill hole surface received a strain heavy enough to produce nanocrystalline structure. The microhardness of the nanocrystalline region (7.3 GPa) is much higher than the subsurface region with deformed martensite structure (4.0 GPa).
NS can also be produced by wear test. In the present study SKD61 tool was slid against the rod of Fe-0.10C specimen with martensite structur. After sliding wear test, homogeneous contrast layer was observed at the surface of specimen. Figure 6 shows wear tested specimen
Fig. defo at L
3 SEM micrographs after a ball drop test. (a) Fe-0.15C fine grained ferrite and (b) Fe-0.80C lite.
4 SEM micrograph after particle impact rmation. Fe-0.80C pearlite impacted 8 times N2 temperature.
Fig. 5 SEM micrograph after drilling of caburized SCM420H.
after annealing. It is seen that homogeneous structure region at the top surface remains unchanged in contrast to the underneath recrystallized region in which clear grain boundaries are seen. From the unique structure, annealing behavior and microhardness, it is concluded that NS was produced by the present wear test.
Nanocrystallization by Shot Peening
Figure 7 shows SEM micrograph of Fe-3.3Si specimen after USSP and subsequent annealing. The top surface layer of several µm thick shows homogeneous structure without grin boundaries. This suggests that NS was produced by USSP as previously reported. Underneath this NS layer is conventional work-hardened region which turned out to be conventional recrystalllized morphology after annealing. It was noted that the thickness of the nanocrystalline layer produced by USSP is much thinner than that of conventiona